Electronic Supplementary Information
Fabrication of high coverage MASnI3 perovskite films for
stable, planar heterojunction solar cells
Takashi Fujihara,a, b Shinobu Terakawa,c Toshinori Matsushima,c, d Chuanjiang Qin,c, e
Masayuki Yahiro,a, b and Chihaya Adachia, b, c, d, e, *
a)Innovative Organic Device Laboratory, Institute of Systems, Information Technologies
and Nano-technologies (ISIT), 744 Motooka, Nishi, Fukuoka 819-0395, Japan.
b)Fukuoka i3-Center for Organic Photonics and Electronics Research (i3-OPERA), 5-14,
kyudaishinmachi, Nishi-ku, Fukuoka 819-0388, Japan.
c)Center for Organic Photonics and Electronics Research (OPERA), Kyushu University,
744 Motooka, Nishi, Fukuoka 819-0395, Japan.
d)International Institute for Carbon Neutral Energy Research (WPI-I2CNER), Kyushu
University, 744 Motooka, Nishi, Fukuoka 819-0395, Japan
e)Japan Science and Technology Agency (JST), ERATO, Adachi Molecular Exciton
Engineering Project, Fukuoka 819-0395, Japan
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
This journal is © The Royal Society of Chemistry 2017
Fig. S1 Photographs of the perovskite films fabricated with different ratios of toluene
and hexane on the PEDOT:PSS coated glass substrate. The toluene:hexane ratio was
changed from 1.5:1 (a, h) to 1:1.5 (e, l) at different temperatures, namely at 13 °C (LT,
a–e) and at 25 °C (RT, h–l).
Fig. S2 Temporal change of transmittance of the perovskite films during bathing in the
different anti-solvent conditions. The solid and open symbols indicate the temperature of
the anti-solvents, namely 13 °C (LT-) and 25 °C (RT-), respectively. Whether toluene and
hexane (Mix), toluene (T), or hexane (H) was used as the co-solvent was indicated by
circles, squares, or triangles, respectively.
Fig. S3 Scanning electron microscopy (SEM) images and atomic force microscopy
(AFM) images for the different conditions. LT-Mix (a), LT-T (b), and LT-H (c) indicate
using mixed solvent, toluene, and hexane, respectively, at a temperature of 13 °C (LT-).
RT-Mix (d), RT-T (e), and RT-H (f) indicate using mixed solvent, toluene, and hexane,
respectively, at a temperature of 25 °C (RT-). The scales of AFM images were 3 m 3
Table S1 The thickness and surface roughnesses for different anti-solvent conditions.
The Rq indicates the root mean square value.
Fig. S4 Optical densities of perovskite films fabricated with the different anti-solvent
conditions. The solid and open symbols indicate the temperature of the anti-solvents at
13 °C (LT-) and 25 °C (RT-), respectively. Whether toluene and hexane (Mix), toluene
(T), or hexane (H) was used as the co-solvent is indicated by circles, squares, or triangles,
Fig. S5 (a) The X-ray diffraction spectra for the LT-Mix (red), LT-T (blue), LT-H (green),
RT-Mix (orange), RT-T (purple), and RT-H (gray) conditions, as well as the substrate-
only spectrum (Black). The asterisks indicate the peaks originating from the substrate
with the dome type cover, which was employed protect the perovskite film from exposure
to air. The semi-log plots of the data are shown in (b).
Fig. S6 Current–voltage characteristics and incident photon to electron conversion
efficiency (IPCE) for the best performing cell under each anti-solvent condition. (a)
Dark current (i.e., without light illumination). (b, d) Photocurrent measured with (1.8
mm 1.8 mm) and without shadow mask (2 mm 2 mm) under AM1.5 simulated
sunlight of 100 mW/cm2. (c) IPCE spectrum for different anti-solvent conditions.
Fig. S7 Key photovoltaic parameters for different anti-solvent conditions. The measured
and averaged values are indicated by open and solid circles, respectively. The evaluated
number of cells was 20 for LT-Mix and between 4 and 8 for the other condition,
respectively. The average values with their standard deviations are summarized in Table
Table S2 Key photovoltaic parameters for different anti-solvent conditions. The
parameters were measured with the shadow mask in place. The measured number of cells
was 20 for LT-Mix and between 4 and 8 for the other conditions.
Fig. S8 Histograms of the photovoltaic parameters of 20 LT-Mix cells.
Table S3 Comparison of our photovoltaic device results with previously reported
1 T. Yokoyama, D. H. Cao, C. C. Stoumpos, T.-B. Song, Y. Sato, S. Aramaki and M. G. Kanatzidis, J. Phys.,
Chem. Lett., 2016, 7, 776-782.
2 K. P. Marshall, R. I. Walton and R. A. Hatton, J. Mater. Chem. A, 2015, 3, 11631-11640.
3 S. J. Lee, S. S. Shin, Y. C. Kim, D. Kim, T. K. Ahn, J. H. Noh, J. Seo and S. Il Seok, J. Am. Chem. Soc., 2016,
4 W. Liao, D. Zhao, Y. Yu, C. R. Grice, C. Wang, A. J. Cimaroli, P. Schulz, W. Meng, K. Zhu, R.-G. Xiong
and Y. Yan, Adv. Mater. 2016, DOI: 10.1002/adma.201602992.